A theoritical study on spin coating 2014-04-11¢ A theoritical study on spin coating...
Embed Size (px)
Transcript of A theoritical study on spin coating 2014-04-11¢ A theoritical study on spin coating...
Advances in Materials Research, Vol. 2, No. 4 (2013) 195-208
DOI: http://dx.doi.org/10.12989/amr.2013.2.4.195 195
Copyright © 2013 Techno-Press, Ltd.
http://www.techno-press.org/?journal=amr&subpage=7 ISSN: 2234-0912 (Print), 2234-179X (Online)
A theoritical study on spin coating technique
Department of Physics, Benue State University, Makurdi, Nigeria
(Received Jun3 21, 2012, Revised January 03, 2013, Accepted April 8, 2013)
Abstract. A comprehensive theory of the spin coating technique has been reviewed and the basic principles and parameters controlling the process are clearly highlighted, which include spin speed, spin time, acceleration and fume exhaust. The process generally involves four stages: a dispense stage, substrate acceleration stage, a stage of substrate spinning at a constant rate and fluid viscous forces dominate fluid thinning behaviour and a stage of substrate spinning at a constant rate and solvent evaporation dominates the coating thinning behaviour. The study also considered some common thin film defects associated with this technique, which include comet, striation, chucks marks environmental sensitivity and edge effect and possible remedies.
Keywords: substrate; centrifugal force; spin coating; thin film; photolithography; acceleration
Spin coating is a procedure used to apply uniform thin films to flat substrates. A typical process
involves depositing a small puddle of a fluid resin onto the center of a substrate and then spinning
the substrate at high speed (typically around 3000 rpm) (Mitzi et al. 2004). Centrifugal force will
cause the resin to spread to, and eventually off, the edge of the substrate leaving a thin film of resin
on the surface. Final film thickness and other properties will depend on the nature of the resin
(viscosity, drying rate, percent solids, surface tension, etc.) and the parameters chosen for the spin
process. Factors such as final rotational speed, acceleration, and fume exhaust contribute to how
the properties of coated films are defined (Hellstrom 2007, Mitzi et al. 2004). A machine used for
spin coating is called a spin coater, or simply spinner.
Rotation is continued while the fluid spins off the edges of the substrate, until the desired
thickness of the film is achieved. The applied solvent is usually volatile, and simultaneously
evaporates. So, the higher the angular speed of spinning, the thinner the film. The thickness of the
film also depends on the concentration of the solution and the solvent (Hellstrom 2007).
Spin coating is widely used in micro-fabrication, where it can be used to create thin films with
thicknesses below 10 nm. It is used intensively in photolithography, to deposit layers of photoresist
about 1 micrometre thick (Hanaor et al. 2011). Photoresist is typically spun at 20 to 80 revolutions
per second for 30 to 60 seconds. Owing to the low values of thickness which can be achieved
using spin coating methods, this method is often employed in the fabrication of transparent
Corresponding author, Ph.D., E-mail: email@example.com
titanium dioxide thin films on quartz or glass substrates, such thin film coatings may exhibit
self-cleaning and self-sterilizing properties (Hanaor et al. 2011).
One of the most important factors in spin coating is repeatability. Subtle variations in the
parameters that define the spin process can result in drastic variations in the coated film
(Middleman and Hochberg 1993). In spite of few studies regarding to the spin coating method, it
has substantial merits, such as the easy control and handling of chemicals and substrates, and
fabrication of thin film at faster rates (Ilican et al. 2008, Mihi et al. 2006). This study has
considered a comprehensive description of spin coating process and theory, aimed at equipping
intending users of this thin film deposition technique with adequate knowledge to enhance better
2. Description of spin coating process
There are four distinct stages to the spin coating process. These include:
2.1 A dispense stage A typical spin process consists of a dispense step in which the resin fluid is deposited onto the
substrate surface as in Fig. 1(a). Two common methods of dispense are Static dispense, and
Dynamic dispense. Static dispense is simply depositing a small puddle of fluid on or near the
center of the substrate. This can range from 1 to 10 cc depending on the viscosity of the fluid and
the size of the substrate to be coated (Hellstrom 2007, Middleman and Hochberg 1993). Higher
viscosity and or larger substrates typically require a larger puddle to ensure full coverage of the
substrate during the high speed spin step. Dynamic dispense is the process of dispensing while the
substrate is turning at low speed. A speed of about 500 rpm is commonly used during this step of
the process (Hellstrom 2007, Middleman and Hochberg 1993). This serves to spread the fluid over
the substrate and can result in less waste of resin material since it is usually not necessary to
deposit as much to wet the entire surface of the substrate. This is a particularly advantageous
method when the fluid or substrate itself has poor wetting abilities and can eliminate voids that
may otherwise form (Schubert and Dunkel 2003, http://www.holmarc.com/spin_coating_machine.html.
Retrieve on February 18 2013).
2.2 Substrate acceleration stage
This stage is usually characterized by aggressive fluid expulsion from the wafer surface by the
rotational motion (Meyerhofer 1978, Miitzi et al. 2004). Because of the initial depth of fluid on the
wafer surface (Fig. 1(b)), spiral vortices may briefly be present during this stage; these would form
as a result of the twisting motion caused by the inertia that the top of the fluid layer exerts while
the wafer below rotates faster and faster. Eventually, the fluid is thin enough to be completely
co-rotating with the wafer and any evidence of fluid thickness differences is gone. Ultimately, the
wafer reaches its desired speed and the fluid is thin enough that the viscous shear drag exactly
balances the rotational accelerations (Meyerhofer 1978, Miitzi et al. 2004).
Typical spin speeds for this stage range from 1500-6000 rpm, again depending on the
properties of the fluid as well as the substrate. This step can take from 10 seconds to several
http://en.wikipedia.org/wiki/Titanium_dioxide http://www.holmarc.com/spin_coating_machine.html.%20Retrieve%20on%20February%2018 http://www.holmarc.com/spin_coating_machine.html.%20Retrieve%20on%20February%2018
A theoritical study on spin coating technique
Fig. 1 Four distinct stages to spin coating (Hellstrom 2007)
minutes. The combination of spin speed and time selected for this stage will generally define the
final film thickness (Meyerhofer 1978, Miitzi et al. 2004). In general, higher spin speeds and
longer spin times create thinner films. The spin coating process involves a large number of
variables that tend to cancel and average out during the spin process and it is best to allow
sufficient time for this to occur (Meyerhofer 1978, Miitzi et al. 2004).
2.3 A stage of substrate spinning at a constant rate and fluid viscous forces dominate fluid thinning behaviour
This stage is characterized by gradual fluid thinning. Fluid thinning is generally quite uniform (as in Fig. 1(c)), though with solutions containing volatile solvents, it is often possible to see
interference colours “spinning off”, and doing so progressively more slowly as the coating
thickness is reduced (Hanaor et al. 2011). Edge effects are often seen because the fluid flows
uniformly outward, but must form droplets at the edge to be flung off. Thus, depending on the
surface tension, viscosity, rotation rate, etc., there may be a small bead of coating thickness difference around the rim of the final wafer (Hanaor et al. 2011, Meyerhofer 1978). Mathematical
treatments of the flow behaviour show that if the liquid exhibits Newtonian viscosity (i.e., is
linear) and if the fluid thickness is initially uniform across the wafer (albeit rather thick), then the
fluid thickness profile at any following time will also be uniform leading to a uniform final coating
(under ideal circumstances) (Middleman and Hochberg 1993 and Emslie et al. 1958).
2.4 A stage of substrate spinning at a constant rate and solvent evaporation dominates the coating thinning behavior
As the prior stage advances, the fluid thickness reaches a point where the viscosity effects yield
only rather minor net fluid flow. At this point, the evaporation of any volatile solvent species will
become the dominant process (Fig. 1(d)) occurring in the coating. In fact, at this point the coating
effectively “gels”because as these solvents are removed the viscosity of the remaining solution
will likely rise effectively freezing the coating in place (Peeters and Remoortere 2008, Meyerhofer